Research Article  Open Access
Vishal Singh, Shivani Suri, K. K. Bamzai, "Mechanical Behaviour and Fracture Mechanics of Praseodymium Modified Lead Titanate Ceramics Prepared by SolidState Reaction Route", Journal of Ceramics, vol. 2013, Article ID 280605, 9 pages, 2013. https://doi.org/10.1155/2013/280605
Mechanical Behaviour and Fracture Mechanics of Praseodymium Modified Lead Titanate Ceramics Prepared by SolidState Reaction Route
Abstract
The praseodymium modified lead titanate ceramics with composition where = 0.04, 0.06, 0.08, and 0.10 prepared by solidstate reaction technique were subjected to indentation induced hardness testing method. The indentations were induced in the applied load ranging from 0.245 N to 4.90 N. The microhardness varies nonlinearly with load and was best explained by the concept of Newtonian resistance pressure as proposed by Hays and Kendall’s law. Crack propagation, fracture toughness (), brittleness index (), and yield strength () were studied to understand the effect of Pr content on various mechanical parameters. The load independent values were found to increase with the increase in praseodymium content.
1. Introduction
Ceramics are generally associated with distinctive problems, some uniquely beneficial and restrictive which determine the materials utilities, among these are hardness, brittleness, and fracture toughness. The measured hardness of a brittle material as determined by conventional tests (Vickers, Knoop, Rockwell, etc.) is a measure of materials resistance to deformation, densification, displacement and fracture. Conventional hardness measurements, which depend on size of an indentation resulting from an applied load, are load independent. This is especially noticeable at lower indentation loads where most measurements are made in order to avoid experimental problems associated with fracture. Local fracture around and under an indentation can affect the depth of penetration or size of the indentation and thus can be considered an intrinsic part of the indentation process. Fracture can also create practical difficulties in making hardness measurements because cracking at indentation corners or fragmentation can hamper hardness measurements. The degree of fracture at indentations in ceramics is load dependent. Low loads are associated with deformation while fracture is conspicuously more prominent at high loads. Microindentation technology has been used for the measurements of fracture toughness of ceramic materials by Evans and Charles [1]. Generally, the dielectric, piezoelectric, elastic, and mechanical behavior of ferroelectric ceramics depend in a complex way on microstructural parameters such as porosity, grain size, and grain boundary effects. The properties of ferroelectric ceramics are also very sensitive to temperature, to stress and strain, to frequency, and so forth.
Lead titanate (PbTiO_{3}) is well known as a perovskites type ferroelectric material with a high Curie point () of 490°C. A phase transition from the paraelectric cubic phase to the ferroelectric tetragonal phase takes place on decreasing the temperature through the Curie point. Lead titanate (PT) is very difficult to fabricate in the bulk form as they undergo a large volume change on cooling below the Curie point. It is a result of cubic () to tetragonal () phase transformation leading to a strain. Evidence for the existence of internal stress is the observation that sintered pure PT ceramic gradually disintegrates into powder at room temperature due to mechanical breakdown [2]. Therefore, dense PT ceramics were prepared by adding suitable additives or combining with other compounds to form solid solution [3, 4]. The modified PT ceramics are material of interest due to the piezoelectric properties which is due to spontaneous polarization. However, their poor mechanical performance, that is, low bonding strength and low fracture toughness, limits their applications in the field where high strength and high fracture toughness are the important requirement. The piezoelectric, and mechanical properties in modified PT ceramics are important for the use in the generation of high power ultrasonic [1]. The mechanical characteristics of modified PT ceramics are as important as the dielectric, piezoelectric and ferroelectric characteristics. Hence, more and more attention has been focused on understanding and improving the mechanical properties of PT ceramics. This paper reports in a systematic manner, the mechanical characterization of Pr modified lead titanate ceramics using Vickers indentation technique. The relationship between hardness, fracture toughness, brittleness index, yield strength, and their dependence on microstructure and load is also studied. To the best of the author’s knowledge, there is no such report on the Pr modified lead titanate ceramics.
2. Materials and Methods
Praseodymium modified lead titanate (PrPT) ceramics with composition where , 0.06, 0.08, and 0.10 were prepared by solidstate reaction technique. The prepared samples were sintered at temperature 1100°C for 2 h. The lattice parameters were calculated using Xray diffraction pattern whereas microstructural characterization was carried out using electron microscopy, and grain size was measured using the line intercept method, the detail of which has already been reported [5]. In order to study the mechanical characterization, the synthesized material was first of all smoothened by grinding with fine alumina abrasive powder in aqueous medium. To have good reflectivity, necessary for observation under a microscope, the material was then polished with diamond paste on a rotatory polishing machine. Praseodymium modified lead titanate disks of about 10–12 mm in diameter and 2 mm in thickness with optically finished surfaces were used for Vickers microhardness analysis. In the present study, indentation induced microhardness was carried in the load range of 0.245 N to 4.903 N, keeping the indenter at right angles to the surface for 10 seconds in all cases, irrespective of the load. The instrument used is “Auto Detection Microhardness Analyzer” “HMV2” of Shimadzu, Japan. At least five indentations were made on each composition for each load. The distance between any two indentations was kept more than five times the diagonal length of the indentation mark, so as to ensure that surface effects are independent of each other. The diagonal length of each indentation impression was measured, and average diagonal length was computed for calculation. Microhardness was calculated using the formula where “” is the applied load and “” the diagonal length of the indentation mark in micrometers. The error on “” is estimated through the relation: where and ; , and denote errors of , , and , respectively.
For each measurement, only welldefined cracks developed during indentation were considered for a particular indentation impression. The crack length was measured from the centre of indentation mark up to the tip of the crack. A program in Fortran 77, using the method of least squares, was made and run on computer to calculate the values of various parameters.
3. Results and Discussion
3.1. Crystal Tetragonality
Xray diffraction analysis was used for the identification and crystal system of the different compositions of PrPT ceramics. Figure 1 is the Xray diffraction analysis of different PrPT compositions showing single phase tetragonal structure as per JCPDS data no. 06452, whereas Figure 2 shows variation of lattice constants () and crystal tetragonality () with various Pr substitutions. The increase in Pr content decreases the crystal tetragonality (), and it was observed that ratio is always less than 1.064 (the value of pure PbTiO_{3} ceramics). The decrease in the tetragonality with the increase in Pr content clearly indicates that Pr ions enter the lattice on Asite replacing Pb ions resulting in the formation of hard and dense ceramics. A compiled data of lattice constants (), Xray density, experimental density, relative density, and porosity for different composition of Pr substituted in lead titanate is shown in Table 1. It was found that relative density increases from 92.94% to 94.62% of the theoretical density with the increase in praseodymium content. The increase in experimental densities and reduction in porosity is due to the fact that increase in Pr content decreases the tetragonality in PT ceramic, because of its large spontaneous stress described as () [6]. Reduction in internal stress allows the crystallites in grains to accommodate more closely to form a denser microstructure, which results in reduction in porosity and increase in density. From the Xray diffraction pattern, it has been found that as the amount of Pr increases, the main peak 101 shifts towards higher angle as clearly seen in Figure 3, which indicates a decrease in lattice constant [7]. Figure 4 shows one of the representative scanning electron microscopic image with their threedimension view for 8 mole% of PrPT compositions. From the photomicrograph and its threedimension view, one can clearly observe the uniform distribution of the grain in the prepared material, and the grain size varies with compositions and ranges from 268 to 531 nm [5].

3.2. Mechanical Behavior
The dependence of microhardness on the applied load shows different behaviour for different materials. The microhardness is reported to be (i) independent of load [8], (ii) is a function of load [9, 10], and shows complex behavior with change of applied load [11, 12]. The results of indentation induced microhardness studies on PrPT ceramics reveal that microhardness value () decreases nonlinearly as the applied load increases from 0.245 N to 1.961 N in all compositions, and thereafter, the values tend to attain saturation. For 4 mole% of PrPT, the microhardness values ranges from 7239 to 5833 MNm^{−2} in the load ranging from 0.245 to 4.903 N. The hardness value increases with compositions for each applied load, and for 10 mole% of PrPT, the value comes out to be in the range 14486–11604 MNm^{−2} in the load range of 0.245–4.903 N. The behaviour of Vickers microhardness () with applied load for the four different compositions of PrPT is shown in Figure 5. Decrease in microhardness at loads greater than 0.098 N with a trend to stabilize at higher loads is reported in calcium modified lead titanate ceramics [13]. The decrease in microhardness value can be quantitatively explained on the basis of penetration depth of the indentor. Since the indentor penetrates only surface layers at low loads, the effect is more pronounced at these loads. However, as the penetration depth increases, the effect of inner layers becomes more and more prominent, and ultimately there is no change in the value of hardness with load [14, 15]. In the present case, the hardness values get saturated above 1.961 N. This explanation is also favoured by Brookes [16], who associated the hardness increase at low loads with the early stages of plastic deformation. The dependence of hardness with loads in case of different compositions is not in accordance with the Kick’s law [17] where “” is the standard hardness constant and “” is the Meyer’s index (or work hardening coefficient) which is proposed to be equal to 2, implying that the hardness is independent of load. A plot of “” versus “” shown in Figure 6, according to (3), using least square fitting method gives the value of “” and “,” as determined from the slope and intercept, respectively. The value of “” comes out to be 1.86, 1.84, 1.86, and 1.85 for 4, 6 8, and 10 mol% compositions, respectively. In each case, the value of is less than 2. The value of in the case of those materials where hardness decreases with load [18] which is also consistent with our observations. In the low load region, resistance offered by the material may be comparable with applied load, resulting in higher values of hardness.
Hardness is defined as the ability of a body to resist permanent deformation and is expressed as the ratio of load applied to the area of indentation. This does not necessarily imply that the applied pressure actually acts on the specimen. According to Hays and Kendall’s law [19], it is assumed that the applied load “” is partially affected by small resultant pressure “,” which is a function of material under investigation. “” is thus the minimum applied load required to cause a plastic deformation. Hays and Kendall [19] modified Kick’s law [17] on the basis of sample resistance pressure (). According to them, where “” is a constant and is the logarithmic index. In this case, would be equal to 2, since it is proposed that the factor “” allows the limiting case to prevail where the hardness is not markedly dependent on the load. To evaluate “,” it is feasible to solve (3) and (4) by substituting for from (3) in (4), so as to get or Figure 7 shows a plot of versus for different compositions of PrPT. The value of and is obtained from the slope and intercept of the plots using least square fitting method. Having obtained the value of “” from Figure 6, the value of “” and “” is calculated for the different compositions of PrPT and is given in Table 2. A plot of “” versus “” shown in Figure 8 yields the value of , thereby suggesting the validity of the theory involving concept of resistance pressure () as proposed by Hays and Kendall’s law.
 
represents the value of Mayer’s index “” on operation of Kick’s law (). represents the value of Mayer’s index “” on operation of Hays and Kendall’s law () = . 
The application of Hays and Kendall’s law lead us to a formula which gives load independent value of : or
Equation (8) gives the microhardness value independent of load. Thus, microhardness value as calculated by using (8) for 4, 6, 8, and 10 mole% of PrPT comes out to be 6018, 6237, 9704, and 11566 MN/m^{2}, respectively.
The microhardness value decreases initially as the load increases and tends to attain saturation at loads greater than 1.96 N and continues to remain saturated up to the maximum applied load of 4.903 N as seen in Figure 5. The saturated value of “” is consistent with the load independent value of “” as obtained from (8). The load independent value of hardness is found to increase linearly with praseodymium substitution. Increase in praseodymium substitution reduces lattice tetragonality [20], which results in the formation of hard and dense ceramics. Increase in with decreasing tetragonality has been reported for modified lead titanate ceramics [21]. These results attributed to internal stresses induced in the sample on cubictetragonal phase transition. Tickoo et al. [22] and Yamamoto et al. [23] have reported decrease of crystal tetragonality as the lanthanum content in PT ceramics increases. They have further observed that the decrease in tetragonality increases Vickers hardness, thereby suggesting that as the praseodymium content increases, the Vickers hardness is expected to increase. It is further supported by the observations made by Okazaki [24].
3.2.1. Yield Strength
From the hardness values, the yield strength “” can be calculated [25]. For Meyer’s index ,
As the values of “” for each composition of praseodymium modified lead titanate is found to be less than 2, therefore, (9) is applied in the present case. Yield strength for 4 mole% is found to have values varying from 2410 to 1944 MNm^{−2} for 6 mole%, 2921 to 2074 MNm^{−2}, for 8 mole%, 3952 to 3331 MNm^{−2}, and for 10 mole% the value varies from 4828 to 3868 MNm^{−2} under the load range from 0.245 to 4.903 N respectively.
3.3. Fracture Mechanics
3.3.1. Fracture Toughness
Resistance to fracture indicates the toughness of a material. The indentation load for crack initiation reflects the intrinsic deformation and fracture properties of the material [26, 27]. The crack developed on a crystal determines the fracture toughness “,” which in turn tells us how much fracture stress is applied under uniform loading. The fracture toughness is an important parameter for the selection of materials for application where the load exceeds the limit or yield point. The fracture toughness value depends on the type of crack system and is given by Ponton and Rawlings [28]. Generally, the fracture toughness “” measured by microindentation technique is expressed as where “” is the applied load in Newton, “” is the crack length measured from the center of indentation mark to crack end (in μm), and “” is the numerical constant that depends upon the indenter geometry. For a Vickers indenter, “” is equal to 7. However, the analysis based on (10) yields reliable values of the fracture toughness only if ; that is, when the crack system is median or halfpenny, where “” is the length of the halfdiagonal of the indent. For (when crack system is Palmqvist type), the values of “” appear less satisfactory [29, 30]. The fracture toughness values for Palmqvist type of crack system may be calculated by generalized Palmqvist equation [28, 30] as where is the mean Palmqvist crack length.
In the present studies, it was observed that the cracks become prominent and measurable at applied load of 0.98 N and above. Figure 9 shows the representative photomicrograph of indentation marks and cracks associated with them at an applied load of 1.961 N for all the four compositions of Pr modified lead titanate. The crack length increases as the applied load increases for 4, 6, 8, and 10 mole% and is shown in Figure 10, but it is also observed that crack length at a particular load decreases with the increase in Pr substitution which indicates the dependence of crack length on both the applied load and variation of Pr substitution. All the cracks developed in the load ranges from 0.980 to 4.903 N are Palmqvist in nature as in all composition the value of is less than 2.5. Table 3 gives a compiled data regarding the crack length, value of , and nature of cracks associated with the corresponding load. Fracture toughness “” is calculated using (11) and its dependence on applied load for different compositions is shown in Figure 11. Fracture toughness increases with the increase in load and tends to attain saturation at higher loads. Also fracture toughness at a given load is found to increase with the increase in praseodymium substitution.

3.3.2. Brittleness Index
Another important property that affects the mechanical behaviour of a material and reflects an idea about the fracture induced in a material without any appreciable deformation is expressed in terms of brittleness index (). From the value of fracture toughness, brittleness index () can be calculated using the relation proposed by Niihara et al. [30]
Dependence of brittleness index on load for different compositions of PrPT is shown in Figure 12. Brittleness index shows significant dependence on load in low load region for 10 mol% of praseodymium. However, small decrease in in low load region with tendency to achieve saturation at higher loads is observed for other praseodymium modified composition.
4. Conclusion
The experimental density of praseodymium modified lead titanate with compositions where , 6, 8, and 10 mole% increases, and crystal tetragonality () decreases with the increase in Pr content as a result of which there is reduction in porosity. The variation of microhardness with applied load is nonlinear and fits well into the concept of Newtonian resistance pressure as proposed by Hays and Kendall’s law. Application of this law gives load independent values of the microhardness for the 4, 6, 8, and 10 mole% of praseodymium modified lead titanate as 6018, 6237, 9704, and 11566 MNm^{−2}, respectively. The load independent value of microhardness is found to increase linearly with the increase in praseodymium substitution due to the decrease in crystal tetragonality. Welldefined and measurable cracks are associated with the indentation impression at a load of 0.98 N and above. All the cracks are Palmqvist in nature. The crack length increases with the increase in load. However, at a constant load, crack length decreases with increase in praseodymium substitution. The values of fracture toughness () and brittleness index () strongly depend upon the applied load.
Acknowledgment
The authors are thankful to DRDO, New Delhi, India for providing grants under ER/IPR Grant in aid scheme.
References
 A. G. Evans and E. A. Charles, “Fracture toughness determination by indentation,” Journal of the American Ceramic Society, vol. 59, no. 78, pp. 371–372, 1976. View at: Publisher Site  Google Scholar
 Y. Matsuo and H. Saski, “Effect of grain size on micro cracking in lead titanate ceramics,” Journal of the American Ceramic Society, vol. 49, no. 4, pp. 229–230, 1966. View at: Publisher Site  Google Scholar
 T. Y. Tien and W. G. Carlson, “Effect of additive on properties of lead titanate,” Journal of the American Ceramic Society, vol. 45, no. 12, pp. 567–571, 1962. View at: Publisher Site  Google Scholar
 I. Ueda and S. Ikegarni, “Piezoelectric properties of modified PbTiO_{3} ceramics,” Japanese Journal of Applied Physics, vol. 7, no. 3, pp. 236–242, 1968. View at: Publisher Site  Google Scholar
 V. Singh, K. K. Bamzai, S. Suri, and N. Nidhi, “Preparation, structural and electrical characteristics of praseodymium modified lead titanate,” Ceramics International, vol. 37, no. 7, pp. 2655–2662, 2011. View at: Publisher Site  Google Scholar
 T. Takahashi, “Influence of samarium substitution on dielectric properties of barium titanate based ceramics,” Ceramic Bulletin, vol. 69, pp. 691–695, 1990. View at: Google Scholar
 P. Kumar, S. Singh, J. K. Juneja, C. Prakash, and K. K. Raina, “Influence of samarium substitution on dielectric properties of barium titanate based ceramics,” Modern Physics Letters B, vol. 23, no. 28, pp. 3419–3425, 2009. View at: Publisher Site  Google Scholar
 C. Asaheron, C. Huse, G. Kuhn, and H. Neumann, “Microhardness of Sndoped lnP,” Crystal Research and Technology, vol. 24, pp. 33–35, 1989. View at: Google Scholar
 K. Balakrishnan, B. Vengatesan, N. Kanniah, and P. Ramasamy, “Growth and microindentation studies of CulnSe_{2} single crystals,” Journal of Materials Science Letters, vol. 9, no. 7, pp. 785–787, 1990. View at: Publisher Site  Google Scholar
 K. K. Bamzai, P. N. Kotru, and B. M. Wanklyn, “Fracture mechanics, crack propagation and microhardness studies on flux grown ErAlO_{3} single crystals,” Journal of Materials Science and Technology, vol. 16, no. 4, pp. 405–410, 2000. View at: Google Scholar
 P. R. Dhar, K. Bamzai, and P. N. Kotru, “Deformation and microhardness studies on natural apophyllite crystals,” Crystal Research and Technology, vol. 32, no. 4, pp. 537–544, 1997. View at: Google Scholar
 J. Guille and M. Sieskind, “Microindentation studies on BaFCl single crystals,” Journal of Materials Science, vol. 26, no. 4, pp. 899–903, 1991. View at: Publisher Site  Google Scholar
 J. Ricote, L. Pardo, and B. Jiménez, “Mechanical characterization of calciummodified lead titanate ceramics by indentation methods,” Journal of Materials Science, vol. 29, no. 12, pp. 3248–3254, 1994. View at: Publisher Site  Google Scholar
 H. Buckle, “Progress in microindentation hardness testing,” International Materials Reviews, vol. 4, no. 1, pp. 49–100. View at: Publisher Site  Google Scholar
 J. R. Pandya, L. J. Bhagia, and A. J. Shah, “Microhardness of rhombohedral crystals: calcite and sodium nitrate,” Bulletin of Materials Science, vol. 5, no. 1, pp. 79–82, 1983. View at: Publisher Site  Google Scholar
 C. A. Brookes, “The mechanical properties of cubic boron nitridea perspective view,” Institute of Physics Conference Series, vol. 75, pp. 207–220, 1986. View at: Google Scholar
 F. Kick, Das Gesetz der proportionalen Widerstände und seine Anwendungen, Felix, Leipzig, Germany, 1885.
 J. B. Quinn and G. D. Quinn, “Indentation brittleness of ceramics: a fresh approach,” Journal of Materials Science, vol. 32, no. 16, pp. 4331–4346, 1997. View at: Google Scholar
 C. Hays and E. G. Kendall, “An analysis of Knoop microhardness,” Metallography, vol. 6, no. 4, pp. 275–282, 1973. View at: Google Scholar
 R. Tickoo, R. P. Tandon, N. C. Mehra, and P. N. Kotru, “Dielectric and ferroelectric properties of lanthanum modified lead titanate ceramics,” Materials Science and Engineering B, vol. 94, no. 1, pp. 1–7, 2002. View at: Publisher Site  Google Scholar
 P. Duran, J. F. F. Lozano, F. Capel, and C. Moure, “Large electromechanical anisotropic modified lead titanate ceramics. Part 2: dielectric, piezoelectric and mechanical properties,” Journal of Materials Science, vol. 24, no. 2, pp. 447–452, 1989. View at: Publisher Site  Google Scholar
 R. Tickoo, R. P. Tandon, V. K. Hans, K. K. Bamzai, and P. N. Kotru, “Electromechanical and piezoelectric studies of lanthanum modified lead titanate ceramics,” Materials Science and Engineering B, vol. 100, no. 1, pp. 47–52, 2003. View at: Publisher Site  Google Scholar
 T. Yamamoto, H. Igarashi, and K. Okazaki, “Dielectric, electromechanical, optical, and mechanical properties of lanthanummodified lead titanate ceramics,” Journal of the American Ceramic Society, vol. 66, no. 5, pp. 363–366, 1983. View at: Google Scholar
 K. Okazaki, “Microstructure and properties of some electrooptic ceramics,” Ferroelectrics, vol. 49, no. 1, pp. 141–150, 1983. View at: Publisher Site  Google Scholar
 J. R. Cahoon, W. H. Broughton, and A. R. Kutzak, “The determination of yield strength from hardness measurements,” Metallurgical Transactions, vol. 2, no. 7, pp. 1979–1983, 1971. View at: Publisher Site  Google Scholar
 H. Ishikaa and N. Shinkai, “Critical load for median crack initiation in vickers indentation of glasses,” Journal of the American Ceramic Society, vol. 65, no. 8, pp. C124–C127, 1980. View at: Publisher Site  Google Scholar
 B. R. Lawn and A. G. Evans, “A model for crack initiation in elastic/plastic indentation fields,” Journal of Materials Science, vol. 12, no. 11, pp. 2195–2199, 1977. View at: Publisher Site  Google Scholar
 C. B. Ponton and R. D. Rawlings, “Dependence of the vickers indentation fracture toughness on the surface crack length,” British Ceramic, vol. 88, no. 3, pp. 83–90, 1989. View at: Google Scholar
 D. J. Bhat, “Elastic/plastic indentation damage in ceramics: the median/radial crack system,” Journal of the American Ceramic Society C, vol. 64, no. 11, pp. C165–C166, 1981. View at: Publisher Site  Google Scholar
 K. Niihara, R. Morena, and D. P. H. Hasselman, “Evaluation of KIc of brittle solids by the indentation method with low cracktoindent ratios,” Journal of Materials Science Letters, vol. 1, no. 1, pp. 13–16, 1982. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2013 Vishal Singh et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.